Embed Size (px)
Contents lists available at ScienceDirect
Journal of the Mechanics and Physics of Solids
Journal of the Mechanics and Physics of Solids 66 (2014) 42–58
journal homepage: www.elsevier.com/locate/jmps
Thermomechanics of monolayer graphene: Rippling, thermalexpansion and elasticity
Wei Gao, Rui Huang n
Department of Aerospace Engineering and Engineering mechanics, University of Texas, Austin, TX 78712, USA
a r t i c l e i n f o
Article history:Received 15 September 2013Received in revised form1 December 2013Accepted 28 January 2014Available online 15 February 2014
Keywords:GrapheneThermal expansionElasticityMolecular dynamicsStatistical mechanics
x.doi.org/10.1016/j.jmps.2014.01.01196 & 2014 Elsevier Ltd. All rights reserved.
esponding author.ail address: [email protected] (R. Hu
a b s t r a c t
Thermomechanical properties of monolayer graphene with thermal fluctuation are studiedby both statistical mechanics analysis and molecular dynamics (MD) simulations. While thestatistical mechanics analysis in the present study is limited by a harmonic approximation,significant anharmonic effects are revealed by MD simulations. The amplitude of out-of-plane thermal fluctuation is calculated for graphene membranes under both zero stress andzero strain conditions. It is found that the fluctuation amplitude follows a power-law scalingwith respect to the linear dimension of the membrane, but the roughness exponents aredifferent for the two conditions due to anharmonic interactions between bending andstretching modes. Such thermal fluctuation or rippling is found to be responsible for theeffectively negative in-plane thermal expansion of graphene at relatively low temperatures,while a transition to positive thermal expansion is predicted as the anharmonic interactionssuppress the rippling effect at high temperatures. Subject to equi-biaxial tension, theamplitude of thermal rippling decreases nonlinearly, and the in-plane stress-strain relationof graphene becomes nonlinear even at infinitesimal strain, in contrast with classical theoryof linear elasticity. It is found that the tangent biaxial modulus of graphene depends onstrain non-monotonically, decreases with increasing temperature, and depends on mem-brane size. Both statistical mechanics and MD simulations suggest considerable entropiccontribution to the thermomechanical properties of graphene, and as a result thermalrippling is intricately coupled with thermal expansion and thermoelasticity for monolayergraphene membranes.
& 2014 Elsevier Ltd. All rights reserved.
As a two-dimensional crystal membrane, graphene has drawn tremendous interests for research and applications. Among itsmany unique properties, the mechanical properties of graphene combine high in-plane stiffness and high strength (Lee et al.,2008) with extremely low flexural stiffness (Lu et al., 2009), rendering a highly deformable but robust membrane material.Experimental observations have found that suspended graphene membranes often display spontaneous ripples (Meyer et al.,2007; Bangert et al., 2009; Zan et al., 2012). Theoretically, different physical origins for rippling have been proposed. Thompson-Flagg et al. (2009) suggested that the rippling could be a consequence of adsorbed OH molecules on random sites. On the otherhand, thermal fluctuation has been considered as a reasonable explanation for intrinsic ripples in graphene (Fasolino et al., 2007;
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–58 43
Abedpour et al., 2007). In the present study, we focus on the effects of thermal fluctuation on thermomechanical properties ofmonolayer graphene, including thermal expansion and temperature-dependent elastic modulus.
The basic mechanical properties of graphene have been reasonably understood, including elastic moduli for in-planeextension and bending. However, the effect of temperature on the mechanical properties of graphene is not well understood.The fact that the elastic moduli measured at the room temperature (T�300 K) are in close agreement with theoretical valuespredicted at T¼0 K may imply insignificant temperature dependence for the elastic moduli. By molecular dynamics (MD)simulations, Zhao and Aluru (2010) predicted that Young's modulus of graphene does not vary significantly with temperatureup to about 1200 K, beyond which graphene becomes more compliant. On the other hand, by means of atomistic Monte Carlo(MC) simulations, Zakharchenko et al. (2009) predicted a non-monotonic behavior of shear modulus of graphene with amaximum at about 900 K, and Chen and Chrzan (2011) predicted monotonic decrease of the elastic modulus of graphenewith temperature up to 4000 K. Since graphene spontaneously fluctuates out-of-plane at a finite temperature, the effective in-plane elastic modulus is expected to depend on the significance of thermal fluctuation. Another manifestation of out-of-planethermal fluctuation is possible reduction of the projected area, which has been suggested as the cause for negative in-planethermal expansion of graphene (Zakharchenko et al., 2009; Chen and Chrzan, 2011). Based on density-functional-theory (DFT)calculations and a quasiharmonic approximation (QHA), Mounet and Marzari (2005) predicted negative in-plane thermalexpansion for graphite and graphene, which was attributed to the lowest transversal acoustic (ZA) phonon modes (also calledbending modes). Negative thermal expansion of graphene was also predicted by a nonequilibrium Green's function approach(Jiang et al., 2009) and ab initio molecular dynamics (AIMD) simulations (Pozzo et al., 2011). Experimentally, Bao et al. (2009)measured thermal expansion of suspended graphene by SEM imaging between 300 and 400 K, with a transition from negativeto positive coefficient of thermal expansion (CTE). Based on frequency measurements of suspended graphene electromecha-nical resonators, Singh et al. (2010) extracted negative CTEs for graphene between 300 and 30 K. Considerable discrepanciesremain between the experimental measurements and theoretical predictions for CTE of graphene.
The present work combines MD simulations of graphene with a statistical mechanics (SM) approach for the study ofthermomechanical properties of monolayer graphene. The SM approach has been used extensively for the study of flexiblemembranes (Bowick and Travesset, 2001; Nelson et al., 2004; Freund, 2013), primarily for biological membranes. Withrelatively simple atomistic structures in graphene, it is possible to directly sample the statistical behavior of graphenemembranes with atomistic details to compare with theoretical SM analysis (Los et al., 2009; Zakharchenko et al., 2010),hence opening a new paradigm for the study of membrane physics. The rest of this paper is organized as follows.A theoretical approach based on statistical mechanics of a continuum elastic membrane is presented in Section 2. Section 3describes the MD simulation method. In Section 4, the results from MD simulations are discussed in comparison with thetheoretical analysis. Section 5 summarizes the results and findings.
2. Statistical mechanics of graphene
2.1. A continuum membrane model
Consider monolayer graphene as a continuum membrane with a two-dimensional (2D) reference configuration in theground state at T¼0 K. The in-plane dimensions of the graphene membrane are much larger than the atomic length scales(e.g., the bond length, r0�0.142 nm), while the monatomic thickness is undefined (and unnecessary) in the continuummodel. The kinematics of general thermomechanical deformation can be described by an in-plane Green–Lagrange straintensor and a curvature tensor, based on a 2D to 3D mapping (Arroyo and Belytschko, 2002; Lu and Huang, 2009). Under theassumption of relatively small deformation but with moderately large out-of-plane deflection, the in-plane strain andcurvature are approximately
� �; ð1Þ
καβ ¼ ∂2w∂xα∂xβ
where the Greek subscript (α or β) represents x or y for the in-plane coordinates, ux and uy are in-plane displacements, and w isout-of-plane deflection. It is noted that the strain tensor in Eq. (1) includes a nonlinear contribution from the out-of-planedeflection that leads to geometric coupling between the in-plane and out-of-plane deformation modes. The kinematics isidentical to the von Karman nonlinear plate theory (Timoshenko and Woinowsky-Krieger, 1987).
The total potential energy of the membrane consists of two parts: in-plane strain energy and bending energy. Under thecondition of small deformation, the strain energy density function can be written as
Φðε;κÞ ¼ΦεðεÞþΦκðκÞ; ð3Þ
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–5844
Φε ¼ E2ð1þνÞ εαβεαβþ ν
� �; ð4Þ
Φκ ¼12DI2κ �DGIIκ ¼
Four elastic constants are used in the above equations, including the 2D Young's modulus E (unit: N/m), Poisson's ratio ν,bending modulus D, and Gaussian curvature modulus DG. They are all defined for the potential energy in the ground state,thus independent of temperature. Note that the bending strain energy density Φκ is written as a function of the twoinvariants of the curvature tensor (Helfrich, 1973): Iκ ¼ κ11þκ22 and IIκ ¼ κ11κ22�κ212; the first invariant is twice of the meancurvature, and the second invariant is Gaussian curvature. In classical plate theory (Timoshenko and Woinowsky-Krieger,1987), both bending moduli (D and DG) can be related to the in-plane Young's modulus and Poisson's ratio. For graphene,however, they are determined from atomistic modeling as independent constants (Koskinen and Kit, 2010; Wei et al., 2012).As discussed in a previous study (Lu et al., 2009), the physical origin of the bending moduli of monolayer graphene isfundamentally different from that in classical plate theory.
As noted by Helfrich (1973) in the study of lipid bilayers, the bending energy due to Gaussian curvature depends solelyon boundary conditions and can be ignored in most cases. Therefore, the total bending energy of a membrane can be writtenas an area integral:
where Ω is the area of the membrane in the reference state. In the present work, we extend the Helfrich membrane modelto study thermomechanical properties of graphene, in comparison with MD simulations.
The mechanical properties of graphene in the ground state (T¼0 K) have been predicted by DFT calculations (Kudin et al.,2001): E¼345 N/m, ν¼0.15, and D¼1.5 eV. However, the empirical potential used in the MD simulations yields differentvalues (Lu and Huang, 2009): E¼243 N/m, ν¼0.397, and D¼1.4 eV. The second set of mechanical properties is used whencomparing the theoretical predictions with MD simulations. Despite the discrepancy in the 2D Young's modulus, thepredictions for the 2D biaxial modulus, En ¼ E=ð1�νÞ, are in close agreement between the empirical potential (En�403 N/m)and DFT (En�406 N/m).
2.2. Out-of-plane thermal fluctuation
Now consider a square-shaped graphene membrane of side length L0 in the ground state. At a finite temperature butsubject to no external force, the membrane fluctuates with both in-plane and out-of-plane modes. In this section weconsider out-of-plane thermal fluctuation only. Assuming periodic boundary conditions, the lateral deflection can be writtenin form of the Fourier series:
wðrÞ ¼∑kwðqkÞeiqk U r; ð7Þ
and the Fourier coefficients are
wðrÞe� iqk U rdΩ; ð8Þ
where r is the 2D position vector in the ground state and qk denotes the k-th wave vector in the 2D space.Substituting Eqs. (7) into (6) and applying the Parseval theorem (Kammler, 2007), we obtain the bending energy of the
membrane in terms of the Fourier coefficients
where qk ¼ jqkj, wReðqkÞ and wImðqkÞ are the real and imaginary parts of wðqkÞ, respectively.For a statistical treatment, wReðqkÞ and wImðqkÞ are taken as continuous random variables. Each set of wReðqkÞ and wImðqkÞ
constitutes a possible configuration of the membrane. All possible configurations of the membrane construct a statisticalensemble. It is important to note that the Fourier coefficients wðqkÞ and wð�qkÞ are not independent. Since w(r) is real-valued in Eq. (8), it can be shown that
wReðqkÞ ¼ wReð�qkÞ and wImðqkÞ ¼ �wImð�qkÞ: ð10Þ
Consequently, only those Fourier coefficients associated with the upper half-plane of the wave vectors (i.e., qk UeyZ0,including only half of the x-axis) are taken as independent random variables. It then follows that the bending energy in
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–58 45
Eq. (9) can be written in terms of the independent random variables as
Ub ¼DL20 ∑kðqk Uey Z0Þ
where ey is the unit vector in the positive direction of y-coordinate.For each possible configuration, the total potential energy is
where Us ¼∬ΩΦεðεÞdΩ. Under the assumption of small deflection, the nonlinear contribution to the in-plane strain in Eq. (1)is neglected. Consequently, the in-plane strain energy Us is independent of the out-of-plane fluctuation, and the in-planeand out-of-plane modes are decoupled. This is commonly taken as a harmonic approximation.
Based on classical statistical mechanics (Pathria, 1996; Weiner, 2002), the probability density function (PDF) for eachconfiguration is given by Boltzmann distribution at thermal equilibrium:
ρ¼ 1Zexp � U
� �; ð13Þ
where kB is the Boltzmann constant, T is the temperature, and Z is the configurational partition function. The partitionfunction is calculated by an integral with respect to all independent random variables (including both the in-plane and out-of-plane modes) for all possible configurations. Under the harmonic approximation, the partition function is simply aproduct of two parts, namely
Z ¼ ZbZs; ð14Þ
where the contribution due to the out-of-plane modes is
Zb ¼Z 1
�1exp � Ub
¼ ∏kðqk Uey Z0Þ
�1exp � DL20
¼ ∏kðqk Uey Z0Þ
and Zs is due to the in-plane modes (independent of the out-of-plane fluctuation). The range of each random variable in Eq.(15) has been taken to be from �1 to1 in order to obtain the analytical expression for the partition function. However, theformulation of the bending energy in Eq. (6) assumes moderately large deflection, requiring the fluctuation amplitude to beless than a fraction of its wavelength for each Fourier mode. Nevertheless, Eq. (15) offers a simple but reasonableapproximation, considering that the exponential integrant decays rapidly with the variables. In other words, the large-amplitude fluctuations are statistically suppressed due to the large potential energy (hence low probability density).
With the probability density function in Eq. (13), the mean-square of each Fourier coefficient of the out-of-planefluctuation can be calculated as
�1jwðqkÞj2exp � Ub
� �dwReðq1ÞdwImðq1Þ⋯¼ kBT
Alternatively, by the equi-partition theorem (Pathria, 1996), each independent harmonic term in Eq. (11) has an averageenergy of kBT/2, namely
which leads to the same result as Eq. (16).For each possible configuration, the mean-square amplitude of the out-of-plane fluctuation in the real space is
h2 ¼ 1
Therefore, the expectation value of the mean-square amplitude is
DL20∑kq�4k : ð19Þ
For the square-shaped membrane with periodic boundary conditions, the smallest possible wave number is:qmin ¼ 2π=L0, which depends on the membrane size (L0). The summation in Eq. (19) can then be written in a discrete
0 20 40 60 80 10010-2
n = L0/b
ε0 = 0.1%
ε0 = 0
ε0 = 1%
0 0.5 1 1.5 2
5 nm10 nm20 nm
-1.5 -1 -0.5 0 0.5 1 1.50
hc/L0 = 0.005
Fig. 1. (a) Convergence of the double-series summations in Eqs. (20) and (28), in comparison with the integral approximation (dashed lines) in Eqs. (21)and (29) for L0¼20 nm; (b) dependence of the coefficient γn1 on pre-strain for different membrane sizes (dashed lines by integration); (c) effect of pre-strain on RMS amplitude of out-of-plane thermal fluctuation at T¼300 K by harmonic analysis (symbols by summation and lines by integration); (d)critical temperature as a function of the normalized pre-strain, EnL20ε0=4π
2D, for the limit of harmonic analysis.
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–5846
i; j¼ �n
ði2þ j2Þ�2 ¼ γnkBT16π4D
where γn is a dimensionless coefficient and n¼ qmax=qmin ¼ L0=b, with qmax ¼ 2π=b being the largest possible wave numberand b the smallest physically permissible length scale (e.g., a microscopic cut-off). Alternatively, Helfrich and Servuss (1984)suggested that the summation in Eq. (19) can be converted to an integral as a continuum approximation:
� �2 Z qmax
where L0bb has been assumed to simplify the result. A comparison between Eqs. (20) and (21) would lead to γn-π forn-1. However, as shown in Fig. 1a, the discrete summation in Eq. (20) converges to a larger value, γn-6:026 (for zerostrain), nearly twice of the integral approximation. The discrepancy results from the singular behavior of q�4
k as qk-0.As a typical measure of surface roughness, the root-mean-square (RMS) amplitude of the out-of-plane fluctuation is
which scales linearly with the dimension (L0) of the membrane. Similar results were obtained for thermal fluctuation of fluidmembranes (Helfrich and Servuss, 1984). A slightly different derivation is presented here as an introduction to key conceptsin statistical mechanics. Notably, the constant coefficient in Eq. (21) differs from that in Helfrich and Servuss (1984) by afactor of 4, since the integral is evaluated with different limits for the wave number, following the assumption of periodicboundary conditions. Moreover, the integral approximation in Eq. (21) is found to be inaccurate to evaluate the discretesummation in Eq. (20) for the amplitude of out-of-plane fluctuation, although the linear scaling (hpL0) is unaffected.
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–58 47
2.3. Effect of pre-strain
Next we consider thermal fluctuation of a graphene membrane subjected to a biaxial pre-strain ε0, relative to thereference ground state. In addition to the bending energy, the in-plane stretching energy is
� �2" #
� �2" #28<
With the pre-strain held as a constant, the out-of-plane deflection contributes to the local in-plane strain according toEq. (1) and hence the strain energy density of the membrane in Eq. (4). In the presence of a non-zero pre-strain, the leadingterm of the contribution in Eq. (23) becomes quadratic. Again, we ignore the in-plane fluctuation and take Eq. (7) for theout-of-plane fluctuation. As a harmonic analysis, only the quadratic terms in Eq. (23) are retained, and the total stretchingenergy can be written in terms of the Fourier coefficients as
Us ¼ Enε20L20þEnε0L
20 ∑kðqk Uey Z0Þ
Along with the bending energy in Eq. (11), the total potential energy is
U ¼ UbþUs ¼ Enε20L20þL20 ∑
kðqk Uey Z0ÞðDq4kþEnε0q2k Þ w2
h i: ð25Þ
The partition function for the Boltzmann distribution in Eq. (13) is then obtained as a function of the pre-strain andtemperature:
Zðε0; TÞ ¼ exp � Enε20L20
kðqk Uey Z0Þ1þ Enε0
Following the same steps in the previous section, the expectation value of mean square amplitude of the out-of-planefluctuation is obtained as
DL20∑kq�4k 1þ Enε0
γnn ¼ ∑n
i; j¼ �n
ði2þ j2Þ�2 1þ Enε0L20
Similar results were obtained by others for lipid membranes under tension (Helfrich and Servuss, 1984; Lomholt et al.,2011). As shown in Fig. 1a, the double-series summation in Eq. (28) converges for n¼ L0=b-1, i.e., γnn-γn1, which dependson the pre-strain and the membrane size through the dimensionless group, Enε0L
20=ð4π2DÞ. Again, a continuum approxima-
tion can be obtained by converting the summation in Eq. (27) to an integral (Helfrich and Servuss, 1984), which yields
ln 1þ Enε0L20
It can be shown that Eq. (29) reduces to Eq. (21) when the pre-strain ε0-0. As shown in Fig. 1b, the integralapproximation underestimates the coefficient γn1, although the discrepancy is reduced with a positive pre-strain (tension).
As noted in Eq. (23), the presence of a pre-strain leads to a harmonic coupling between the out-of-plane fluctuation and
in-plane stretching. This coupling introduces a length scale, a¼ffiffiffiffiffiffiffiffiffiffiffiD=En
q. As a result, the RMS amplitude of the out-of-plane
fluctuation is no longer scaling linearly with the membrane size, as shown in Fig. 1c. The out-of-plane thermal fluctuation issignificantly suppressed by a positive pre-strain (tension), especially for relatively large membranes. On the other hand,when the pre-strain is negative (compression), it is interesting to note that the harmonic analysis predicts a singular
behavior for the fluctuation amplitude as ⟨h2⟩-1 for ε0-�q2kD=En by Eq. (27), corresponding to a set of critical strains for
buckling instability of the elastic membrane under compression. By Eq. (29), the fluctuation amplitude blows up at the firstcritical strain (qmin ¼ 2π=L0):
εc ¼ � 4π2D
However, the buckling amplitude would remain finite beyond the critical strain if the higher order terms (anharmonic) inEq. (23) are taken into account, a typical task for nonlinear post-buckling analysis left for future studies.
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–5848
Since the harmonic analysis is limited to relatively small fluctuation amplitudes, a boundary line may be drawn in thetemperature–strain panel as shown in Fig. 1d, where a critical value for the fluctuation amplitude, hc=L0 ¼ 0:005, is assumedfor illustrative purpose. In addition to the critical strain for buckling at T¼0 K, a critical temperature at zero strain can bedefined as
Tc ¼ 16π4DγnkB
Therefore, the harmonic analysis for the out-of-plane thermal fluctuation should be restricted to relatively lowtemperatures, with the critical temperature depending on the membrane size and pre-strain. For a monolayer graphenemembrane, the critical strain for buckling is typically very small, around �2� 10�4 for a membrane of size L0¼10 nm.Assuming hc=L0 ¼ 0:005, the critical temperature at zero strain is about 112 K with D¼ 1:5 eV and γn � 6:026.
2.4. Nonlinear thermoelasticity of graphene
By classical theories of statistical mechanics and thermodynamics (Weiner, 2002), the microscopic partition function isrelated to the macroscopic Helmholtz free energy of the system as
Aðε0; TÞ ¼ �kBT ln Zðε0; TÞ: ð32Þ
The equi-biaxial in-plane stress can then be obtained as a thermodynamic conjugate:
� �T: ð33Þ
By this definition, the stress has the same unit as the energy density (per unit area): J/m2, or equivalently, N/m, so-called2D stress as opposed to the conventional 3D stress.
With the partition function in Eq. (26), we obtain that
kðqk Uey Z0ÞðDq2kþEnε0Þ�1; ð34Þ
where the first term is the biaxial stress in the ground state (no thermal fluctuation) and the second term is the entropiccontribution, arising from the tendency of the graphene membrane to increase its entropy (S¼ �∂A=∂T) by out-of-planefluctuation at a finite temperature. The entropic contribution to the stress can be calculated by summation over all Fouriercomponents, namely
~s ¼ EnkBT16π2D
i; j¼ �n
i2þ j2þ Enε0L20
0 20 40 60 80 100-5
n = L0 /b
0 0.5 1 1.5 2
ε0 = 0.1%
ε0 = 0
ε0 = 1%
5 nm10 nm20 nm
Fig. 2. (a) The coefficient ξn in Eq. (35) by summation (symbols) and integration (dashed lines) for L0¼20 nm; (b) the coefficient η1 in Eq. (36) as a functionof pre-strain and membrane size (symbols by summation and lines by integration).
0 10 20 30 40 50-1
20 nm5 nm
0 10 20 30 40 50-10
Fig. 3. (a) In-plane thermal strain predicted by the harmonic analysis for graphene membranes of different sizes; (b) effective coefficient of thermalexpansion for graphene membranes predicted by the harmonic analysis.
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–58 49
It is found that this summation gives an unbounded stress for n-1 even at zero strain (Fig. 2a). On the other hand, thecorresponding elastic modulus is bounded as follows:
~En ¼ ∂s
∂ε0¼ En 1� EnkBTL
i; j¼ �n
i2þ j2þ Enε0L20
n-1En 1� η1EnkBTL
where η1 is a function of the strain and the membrane size through the dimensionless group, Enε0L20=ð4π2DÞ, as shown in
Fig. 2b. When ε0 ¼ 0, η1 ¼ γ1 ¼ 6:026.By converting the summations to integrals, the stress and modulus are obtained approximately as
~s � EnkBT16πD
� �� ln 1þ EnL20
!" #; ð37Þ
~En � En� EnkBT
which agree closely with the summations except for ε0 ¼ 0 (Fig. 2). It is noted that a finite value of ~s depends on both themembrane size L0 and the cutoff length b, while the latter is difficult to justify for the continuum model. In our calculationswe have taken b¼ 4r0 ¼ 0:568 nm, where r0 ¼ 0:142 nm is the equilibrium C–C bond length in graphene. Remarkably,independent of the cutoff, the effective modulus predicted by Eqs. (36) or (38) includes an entropic contribution due to theout-of-plane thermal fluctuation. As a result, the effective modulus of graphene depends on both the temperature and themembrane size. In particular, the harmonic analysis predicts that the biaxial modulus of graphene decreases linearly withtemperature, hence a thermal softening effect. At zero strain, the modulus decreases with increasing membrane size (L0).The size dependence becomes negligible when graphene is pre-stretched with ε0L
20b4π2D=En. These predictions are further
discussed in Section 4, in comparison with MD simulations.In addition to the out-of-plane fluctuation, the in-plane thermal fluctuation, not considered explicitly in the present
study, has an entropic contribution to the stress as well (Weiner, 2002). The total stress may be written approximately as
s¼ Enðε0�α2DTÞþ ~s; ð39Þwhere α2D is the 2D coefficient of thermal expansion (2D-CTE) resulting from anharmonic interactions among in-planephonon modes when the out-of-plane modes are completely suppressed. As shown by MD simulations (Fig. 6b), the 2D-CTEof graphene is nearly a constant (α2D�5.51�10�6 K�1), independent of temperature or membrane size.
By setting the total stress to zero in Eq. (39), we obtain a nonlinear equation
i; j¼ �n
i2þ j2þ Enε0L20
¼ α2DT ; ð40Þ
which can be solved to predict the in-plane thermal strain, εT ¼ ε0ðs¼ 0Þ, as a function of four dimensionless groups, α2DT ,D=kBT , E
nL20=D, and n. Fig. 3a plots the thermal strain versus temperature for different membrane sizes. Without out-of-planethermal fluctuation, the in-plane thermal strain increases linearly with temperature (� α2DT). The thermal strain issignificantly reduced with out-of-plane thermal fluctuation. Since the amplitude of thermal fluctuation depends on the
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–5850
membrane size, the reduction of thermal strain also depends on the membrane size. The thermal strain remains positive fora small membrane (L0¼3 nm), but becomes negative for larger membranes. By setting ε0 ¼ 0 in Eq. (40), the criticalmembrane size is predicted to be around 4.5 nm. Evidently, the in-plane contraction due to out-of-plane thermal fluctuationof the large membranes (L044.5 nm) outweighs the positive expansion due to the in-plane modes, resulting in aneffectively negative thermal expansion for graphene. Fig. 3b plots the effective in-plane CTE of graphene defined as
� �s ¼ 0
which depends on both the temperature and the membrane size due to the effect of out-of-plane fluctuation. We note thatthe harmonic approximation in the present analysis is limited to low temperatures for relatively large membranes. Beyond acritical temperature, no meaningful solution to Eq. (40) can be found, and anharmonic effects must be taken into account inorder to predict the thermal expansion. Moreover, the harmonic approximation tends to overestimate the in-planecontraction, as discussed in Section 4.
2.5. Anharmonic effects
Theoretical studies of flexible membranes beyond the harmonic approximation have predicted that anharmonic couplingbetween bending and stretching modes could significantly suppress thermal fluctuation. Considering anharmonic effectswith contributions from nonzero Gaussian curvatures, Nelson and Peliti (1987) predicted a power-law scaling for the meanamplitude of thermal fluctuation with respect to the linear dimension of a nearly flat elastic membrane: h� Lζ , where ζ iscalled the roughness exponent: ζ¼ 1 by the harmonic approximation while ζ¼ 0:5 by Nelson and Peliti (1987). However,there is some uncertainty on the precise theoretical value of the roughness exponent, ranging from 0.5 to 0.775 for variousmembrane models (Lipowsky and Girardet, 1990; Abraham and Nelson, 1990; Gompper and Kroll, 1992; Le Doussal andRadzihovsky, 1992; Kownacki and Mouhanna, 2009). With nonlinear coupling between the out-of-plane fluctuation and in-plane displacements, analytical approximations and numerical treatments are required for anharmonic analysis, whichremains a challenging subject. Moreover, the continuum membrane model with energy functionals such as Eqs. (6) and (23)are limited to relatively small fluctuation amplitude and in-plane strain. These limitations can be lifted by discrete atomisticmodels of the membrane. By atomistic MC and MD simulations, Los et al. (2009) found the roughness exponent to be around0.575 for graphene. MD simulations by Abedpour et al. (2007) predicted a temperature dependent roughness exponent inthe range 0:6oζo0:74 for T¼0–700 K. The anharmonic effect on thermal fluctuation is expected to have a profoundinfluence on the thermomechanical properties of graphene. As predicted by atomistic modeling and simulations(Zakharchenko et al., 2009; Chen and Chrzan, 2011), the elastic modulus of graphene depends on the temperature andthe in-plane thermal expansion changes from negative to positive as the temperature increases. In the present study, bycomparing numerical results from MD simulations with theoretical predictions under the harmonic approximation, weemphasize the intimate relationship between thermal rippling and thermoelasticity of graphene with both harmonic andanharmonic effects. Moreover, the statistical nature of thermal rippling renders an entropic contribution to thermo-elasticity; similar entropic effects have been well known for many other materials, including isolated molecular chains(Marko and Siggia, 1995), biological membranes (Safran, 1994), and molecular networks (Treloar, 1958; Su and Purohit,2012).
3. Molecular dynamics simulation
We perform MD simulations of monolayer graphene using LAMMPS, an open source code (Plimpton, 1995). The second-generation reactive empirical bond-order (REBO) potential (Brenner et al., 2002) is used for the multibody C–C interactions
Fig. 4. Snapshots of thermal rippling of a graphene membrane by MD simulations with L0¼20 nm and T¼300 K. (a) and (b) for NPT with zero stress; (c)and (d) for NVT with zero strain. Color bars show out-of-plane deflection of atoms in Å. (For interpretation of the references to color in this figure legend,the reader is referred to the web version of this article.)
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–58 51
in graphene. Square-shaped graphene membranes of different linear dimensions are simulated at finite temperatures withperiodic boundary conditions. The temperature is controlled by a Nose-Hoover thermostat. Each simulation runs up to 40 ns(time step: 1 fs), with the first 10 ns for the system to equilibrate and the subsequent 30 ns for calculations of the time-averaged quantities. The time integration scheme closely follows the time-reversible measure-preserving Verlet and rRESPAintegrators derived by Tuckerman et al (1992). The statistical errors are estimated by fifteen different sets of data, each overa time interval of 2 ns. To simulate monolayer graphene without interlayer interactions, relatively thick simulation boxes areused (thickness 420 nm). VMD, an open source visualization package (Humphrey et al., 1996), was used to generatesnapshots of graphene membranes (Fig. 4).
MD simulations with both constant pressure (NPT) and constant volume (NVT) ensembles are performed. In NPTsimulations, the dimensions of the simulation box are allowed to change to maintain a constant pressure (or stress).In particular, we are interested in zero-pressure (or zero-stress) NPT simulations for freestanding graphene membranes,with which the change of the in-plane dimension is calculated as a function of temperature to predict the in-plane CTE ofgraphene, namely
αðT ; L0Þ ¼1L0
� �; ð42Þ
where L0 is the linear dimension of the graphene membrane in the ground state (T¼0 K) and ⟨L⟩t denotes time average ofthe linear dimension at a finite temperature. On the other hand, the NVT ensemble is used to simulate graphene subjected toa pre-strain (ε0). In such simulations, the dimensions of the simulation box are fixed as L¼ L0ð1þε0Þ, while the in-planereaction stress is evaluated as a function of the pre-strain and temperature by time-averaged virial stress (Admal andTadmor, 2010):
r¼ � 1
Fij � ðri�rjÞþ1
L2∑imivi � vi
where Fij is the interatomic force between two atoms (i and j), ri is the position vector of i-th atom, vi is the velocity vector,mi is the atomic mass, and ⟨U⟩t denotes time average of the enclosed quantity. The virial formula is modified to yield the 2Dstress for graphene, consistent with the definition of stress in Eq. (33).
In both NPT and NVT simulations, the mean amplitude of the out-of-plane thermal fluctuation is calculated by a timeaveraged RMS, namely
i ¼ 1
vuut ; ð44Þ
where N is the total number of atoms and wi is the out-of-plane displacement of i-th atom. Based on the ergodic hypothesis(Weiner, 2002), the time average (over a sufficiently long period) from MD simulation is equivalent to the ensemble averagein statistical mechanics. Consequently, the numerical results from MD simulations can be compared directly with thepredictions based on statistical mechanics.
Moreover, we perform special 2D-MD simulations to study the behavior of graphene membranes in the absence of out-of-plane thermal fluctuation. For a 2D-MD simulation, the out-of-plane components of velocities and forces are zeroed outfor all atoms in every time step. As a result, the graphene membrane remains perfectly flat, but with in-plane fluctuations.It is found that the computational cost and statistical error of 2D-MD are drastically reduced in comparison with regular MD.Each simulation is sufficiently equilibrated by running to 5 ns with a time step of 1 fs. Through these 2D-MD simulations, weobtain a 2D-CTE (α2D�5.51�10�6 K�1) and biaxial stress-strain relation without out-of-plane thermal fluctuation.A comparison with the regular MD simulations would then reveal the effects of out-of-plane thermal fluctuation.
4. Results and discussion
4.1. Thermal rippling
Fig. 4 shows snapshots of a graphene membrane from MD simulations. The out-of-plane thermal fluctuation leads todynamic thermal rippling under both NPT and NVT conditions. The time averaged RMS amplitude of thermal rippling isplotted in Fig. 5, as a function of temperature and membrane size. The rippling amplitude under the zero-stress NPTcondition compares closely with previous studies (Fasolino et al., 2007; Los et al., 2009). Compared to the prediction by theharmonic analysis, the rippling amplitude is considerably lower, suggesting significant anharmonic effect, especially at hightemperatures and for large membranes. Under the zero-strain NVT condition, the rippling amplitude is even lower. This canbe understood as a result of the reactive tensile stress that is required to hold the in-plane dimension of the membrane,as discussed further in Section 4.2. A common assumption in the studies of flexible membranes is inextensibility of thein-plane dimension (Helfrich and Servuss, 1984). Such an assumption would erroneously predict zero out-of-plane
Fig. 5. (a) RMS amplitude of thermal rippling of a graphene membrane (L0¼20 nm) as a function of temperature, from MD simulations under zero-stressNPT and zero-strain NVT conditions. (b) Rippling amplitude as a function of membrane size at T¼300 K, fitted by the scaling law, hpLζ0, with differentroughness exponents for NPT and NVT ensembles.
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–5852
fluctuation under the zero-strain condition. Evidently, in-plane extension is inevitable at a finite temperature despite thehigh in-plane stiffness of graphene.
In Fig. 5b, the rippling amplitude as a function of the membrane size is fitted by the power law, h� Lζ , which yields tworoughness exponents, ζ ¼ 0:67 for NPT (zero stress) and ζ¼ 0:45 for NVT (zero strain), both at T¼300 K. The NPT roughnessexponent agrees well with a previous study (Abedpour et al., 2007), which is also close to the theoretical predictions forother flexible membranes (Lipowsky and Girardet, 1990; Abraham and Nelson, 1990; Gompper and Kroll, 1992; Le Doussaland Radzihovsky, 1992; Kownacki and Mouhanna, 2009). The lower roughness exponent under the zero-strain NVTcondition suggests that the scaling law sensitively depends on the boundary constraint. As predicted by the harmonicanalysis in Fig. 1c and MD simulations (Fig. 7a), a small positive pre-strain could suppress rippling amplitude considerablyand result in very different scaling behavior. Experimentally, when a graphene membrane is suspended over a hole or trench(Meyer et al., 2007; Bangert et al., 2009; Zan et al., 2012), a positive pre-strain or tension is likely imposed due to theadhesive interaction between graphene and the side wall of the hole/trench (Lee et al., 2008; Bunch, et al., 2008; Lu andDunn, 2010). Furthermore, change of temperature would lead to thermal stress in graphene due to thermal expansionmismatch. While a tensile thermal stress would suppress thermal rippling, a compressive thermal stress could lead to staticrippling by buckling instability (Bao et al., 2009). Therefore, the dependence of rippling amplitude on temperature couldbe coupled with thermal expansion induced stress in suspended graphene (Kirilenko et al., 2011), further discussed inSection 4.3.
4.2. Thermal expansion
Thermal expansion of a freestanding graphene membrane is studied by MD simulations under the zero-stress NPTcondition. As shown in Fig. 6a, the macroscopic in-plane strain components are calculated by time averaging at differenttemperatures for different membrane sizes, i.e., εx ¼ ⟨Lx⟩t=L0�1 and εy ¼ ⟨Ly⟩t=L0�1, where L0 is the in-plane dimension ofthe square-shaped membrane in the ground state (T¼0 K) whilst Lx and Ly are projected in-plane dimensions at a finitetemperature. The two strain components are nearly identical in all cases, suggesting transversely isotropic thermalexpansion of graphene. Similar to the prediction by the harmonic analysis (Fig. 3a), the thermal strain becomes increasinglynegative as the membrane size increases, which has been attributed to the in-plane contraction as a result of out-of-planethermal fluctuation. Indeed, by suppressing out-of-plane fluctuation, 2D-MD simulations predict linear, positive thermalexpansion (Fig. 6b), independent of the membrane size. A positive 2D-CTE is obtained as α2D ¼ 5:51� 10�6 K�1, whichremains constant up to T¼1000 K. Such a positive thermal expansion can be understood as a result of anharmonicinteractions among in-plane phonon modes (Weiner, 2002). By subtracting the in-plane expansion from the total thermalstrain, i.e., ~ε ¼ ε�α2DT , we obtain the in-plane contraction due to out-of-plane fluctuation, which depends on thetemperature and membrane size (Fig. 6b). In particular, while the in-plane contraction increases monotonically withincreasing temperature, the rate of increase is slowed down at high temperatures due to the anharmonic effect on thermalrippling. Consequently, the total thermal strain turns to become increasingly positive (or less negative) at hightemperatures. The competition between the two effects (in-plane and out-of-plane modes) on thermal expansion ofgraphene leads to a non-monotonic behavior of thermal strain (Fig. 6a), except for very small membrane size (e.g., 3 nm).A previous study based on quasi-harmonic approximation (QHA) predicted monotonic decreasing of the in-plane latticeparameter of graphene (Mounet and Marzari, 2005), which may have underestimated the anharmonic effects and thusoverestimated the in-plane contraction at high temperatures. More recently, atomistic MC simulations by Zakharchenkoet al. (2009) showed non-monotonic change of the in-plane lattice parameter of graphene, similar to the thermal strain inFig. 6a.
0 200 400 600 800 1000-1
0 200 400 600 800 1000-10
2D MD (no rippling)
0 200 400 600 800 1000-10
, α (1
α2D = 5.51x10-6
Mounet and Marzari (2005)
Jiang et al. (2009)
MD (L0 = 3, 5,10, 20, 30 nm)
0 200 400 600 800 1000-0.4
Fig. 6. (a) In-plane thermal strain of graphene by MD simulations under the zero-stress NPT condition, as a function of temperature for differentmembrane sizes. Squares and circles are for strain components in the armchair and zigzag directions, respectively; error bars are shown for L0¼10 nmonly; solid curves are fourth-order polynomial fittings. (b) Linear, positive thermal expansion of graphene by 2D-MD simulations and the in-planecontraction strain due to out-of-plane thermal fluctuation. (c) Coefficient of thermal expansion of graphene as a function of temperature, comparing MDsimulations with two previous studies. (d) In-plane thermal stress of graphene under zero-strain NVT condition, where the red dashed line shows theprediction by the harmonic analysis for L0¼30 nm.
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–58 53
The nonlinear dependence of the thermal strain on temperature is fitted by a polynomial function (solid lines in Fig. 6a),with which the in-plane CTE of graphene is calculated as a function of temperature for different membrane sizes (Fig. 6c).For a relatively large membrane, the calculated CTE is negative below a critical temperature but becomes positive at highertemperatures. The critical temperature varies from around 100 to 500 K for the membrane size ranging from 3 to 30 nm. Thetransition from negative to positive CTE can also be understood as a result of the competition between the in-plane and out-of-plane modes. In comparison, similar transition to a positive CTE was predicted by Jiang et al. (2009) using a non-equilibrium Green's function method, while the CTE predicted by Mounet and Marzari (2005) remains negative up toT¼2000 K. Experimentally, Bao et al. (2009) reported a transition temperature at around 350 K, close to the present MDresults. While quantitative discrepancies remain to be resolved by more accurate experimental measurements, theprediction for the negative-to-positive transition of CTE is theoretically plausible for graphene, considering the anharmoniceffect on thermal rippling. Such transition of CTE has been also predicted and confirmed experimentally for graphite(Mounet and Marzari., 2005), where the out-of-plane thermal fluctuation is confined by interlayer van der Waalsinteractions.
We note that the in-plane CTEs of graphene obtained from MD simulations increase monotonically with temperature.In contrast, decreasing of CTE was predicted by both QHA (Mounet and Marzari, 2005) and Green's function method (Jianget al., 2009). This discrepancy is largely attributed to the inaccuracy of MD simulations at very low temperatures (To100 K),when the dimensional change is relatively small and thus the thermal strain cannot be accurately determined. Moreover, itis known in solid state physics that quantum effect dominates the low-temperature behavior for specific heat and thermalexpansion (Ashcroft and Mermin, 1976), which is not accounted for in the classical MD simulations. Interestingly, theharmonic analysis in Section 2 does predict decreasing CTEs for relatively large membranes (Fig. 3b), despite the limitedtemperature range. However, the coincidence may not be physically justifiable without taking into account the quantumeffect at low temperatures.
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–5854
With a negative CTE below the transition temperature, a tensile stress is expected for a graphene membrane when its in-plane dimension is fixed. Indeed, as shown in Fig. 6d, the in-plane reaction stress calculated from MD simulations under thezero-strain NVT condition is positive at low temperatures and reaches a peak at around the transition temperature.However, since the amplitude of thermal rippling is lower under the zero-strain condition (Fig. 5a), the CTE of grapheneobtained under the zero-stress NPT condition cannot be used directly to predict the thermal stress here. On the other hand,by setting ε0 ¼ 0 in Eq. (39), the harmonic analysis would predict the thermal stress to be linearly dependent on temperature(dashed line in Fig. 6d), overestimating the stress considerably. Therefore, the anharmonic effect on thermal rippling ofgraphene is intricately coupled with thermal expansion and thermal stress, resulting in a generally nonlinear thermo-mechanical behavior of graphene.
Assuming linear elasticity in the ground state (T¼0 K), a nonlinear stress–strain behavior is predicted at a finitetemperature (T40 K) by the statistical mechanics approach in Section 2 (Eq. 39), including an entropic contribution to thestress due to out-of-plane thermal fluctuation. This behavior is in contrast to the classical theory of linear thermoelasticity,where the total strain is taken as linear superposition of elastic strain and thermal expansion. For graphene, however, thethermal expansion cannot be determined independently from elastic strain (or stress), largely due to thermal rippling andits dependence on strain (or stress) as discussed in Section 4.2. While the harmonic analysis in Section 2 is limited for itsown applicability, the nonlinear thermoelasticity of graphene is confirmed by MD simulations beyond the harmonic regime.By imposing an equi-biaxial in-plane strain under the NVT condition, the corresponding stress in graphene is calculated as afunction of the strain and temperature. Meanwhile, the RMS amplitude of rippling is also calculated to show its effect on thestress–strain relation. As shown in Fig. 7a for a graphene membrane with L0¼20 nm at 300 K, the ripple amplitudedecreases with increasing strain. Compared to the prediction by the harmonic analysis, Eq. (27), the rippling amplitude fromMD is considerably lower around zero strain, due to the anharmonic effect as discussed in Section 4.1. With increasingpositive strain, the MD results compare closely with the harmonic prediction, suggesting that the anharmonic effect issuppressed by the tensile strain. Fig. 7b shows the stress–strain curve for the same membrane. For comparison, a stress–strain curve is also obtained from 2D-MD simulations in absence of any out-of-plane fluctuation. The difference between the
0 0.5 1 1.5 2-1
MD (with ripples)2D-MD (no ripples)
0 0.5 1 1.5 20
MD Harmonic Analysis
0 0.5 1 1.5 2150
MD (with ripples)2D-MD (no ripples)Harmonic analysis
Fig. 7. (a) RMS amplitude of rippling as a function of biaxial strain for a graphene membrane (L0¼20 nm) at T¼300 K, comparing the results from MDsimulations with prediction by the harmonic analysis. (b) Stress–strain curves from MD simulations with and without rippling. (c) Entropic contribution tothe stress as a function of strain. (d) Biaxial modulus as a function of strain.
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–58 55
two stress–strain curves is attributed to the entropic contribution from rippling, as shown in Fig. 7c, in comparison with theprediction in Eq. (35) by the harmonic analysis. Similar to the rippling amplitude in Fig. 7a, the harmonic analysisoverestimates the entropic contribution at zero strain, but becomes reasonably good with a positive strain.
With the stress–strain curves in Fig. 7b, the tangent biaxial modulus of graphene is calculated by numericaldifferentiation as shown in Fig. 7d. Even without out-of-plane fluctuation, the biaxial modulus obtained from 2D-MDsimulations is not a constant, decreasing with increasing strain. Such a nonlinear elastic behavior has been predictedpreviously by both DFT (Wei et al., 2009) and MM calculations (Lu and Huang, 2009; Lu et al., 2011) at T¼0 K, which isnearly independent of temperature and hence considered intrinsic. With out-of-plane fluctuation, the elastic modulus issignificantly lower at small strain. As predicted by the harmonic analysis in Section 2.4, the out-of-plane fluctuation reducesthe effective elastic modulus in Eqs. (36) or (38). The amount of reduction, ΔEn ¼ En� ~E
, decreases with increasing strain,which is a result of decreasing ripple amplitude. Consequently, the elastic modulus first increases with strain (i.e., strainstiffening) as the ripple amplitude decreases. As the rippling effect diminishes with further increasing of strain (40.5%), theintrinsic nonlinear elasticity takes over so that the elastic modulus decreases, following closely the results from 2D-MDsimulations or the ground-state behavior. Therefore, the nonlinear elasticity of graphene at a finite temperature results fromtwo physical origins, one intrinsic (independent of temperature) and the other owing to out-of-plane fluctuation for T40 K.The competition between the two effects results in a non-monotonic dependence of the tangent elastic modulus ofgraphene on strain (Fig. 7d), even at the infinitesimal strain level. For comparison, the elastic modulus predicted by theharmonic analysis is plotted in Fig. 7d, using the elastic modulus from 2D-MD in place of En in Eq. (36). Evidently, themodified harmonic prediction agrees well with the MD results for a relatively large strain (40.5%), but less so near zerostrain.
The effect of out-of-plane fluctuation leads to temperature and size-dependent elastic properties for graphene. As shown inFig. 8a, the stress–strain curves of a graphene membrane with L0¼20 nm are obtained from MD simulations at differenttemperatures at around zero strain (relative to the ground state). At a very low temperature (e.g., T¼10 K), the stress–strain
-0.1 -0.05 0 0.05 0.1
0 K10 K300 K1000 K
0 200 400 600 800 10000
2D MD (no ripples)5 nm10 nm20 nm
Fig. 8. (a) Biaxial stress–strain curves around zero strain for a graphene membrane with L0¼20 nm, obtained from MD simulations at three differenttemperatures, in comparison with the ground-state behavior at T¼0 K from static MM calculations. (b) Tangent biaxial modulus at zero strain as a functionof temperature for different membrane sizes.
0 200 400 600 800 1000280
MD (with ripples)2D-MD (no ripples)Harmonic analysis
0 5 10 15 20280
2D-MD (no ripples)
T = 300K
T = 1000K
Fig. 9. (a) Tangent biaxial modulus at 1% strain as a function of temperature for a graphene membrane with L0¼20 nm, obtained from MD and 2D-MDsimulations, in comparison with the harmonic analysis. (b) Tangent biaxial modulus at 1% strain as a function of membrane size at T¼300 and 1000 K.
300 400 500 600 700 800 900 10000
αs = 0
αs = 1 x 10-6 K-1
αs = 3 x 10-6 K1
αs = 5 x 10-6 K-1
Fig. 10. (a) RMS amplitude of rippling obtained from MD simulations as a function of a temperature for a 20 nm graphene membrane suspended on asubstrate with different CTEs. (b) Biaxial stress versus temperature. The thin dashed lines in (b) are linear prediction of the stress using the properties ofgraphene at T¼300 K (αg¼�0.7�10�6 K�1 and ~E
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–5856
behavior is close to the ground-state behavior at T¼0 K, which can be obtained from the static MM simulation (Lu and Huang,2009). As the temperature increases, the slope of the stress–strain curve decreases, indicating thermal softening in the elasticmodulus. Fig. 8b plots the tangent modulus at zero strain as a function of temperature for three different membrane sizes. Forcomparison, the tangent modulus obtained from 2D-MD is also plotted, showing essentially no temperature dependence withEn ¼ 403:0 N=m, in close agreement with DFT calculations (En�406 N/m) (Kudin et al., 2001; Wei et al., 2009). It is well knownthat elastic modulus of a crystalline solid is in general temperature dependent and in particular, linear temperature dependencehas been predicted under the harmonic approximation (Weiner, 2002). Similarly for graphene, the harmonic analysis in Section 2predicts linear thermal softening of the elastic modulus in Eqs. (36) or (38). However, with significant anharmonic effect at zerostrain, a nonlinear temperature dependence is predicted for the elastic modulus of graphene (Fig. 8b). Moreover, the elasticmodulus of graphene is size dependent: lower modulus for larger membrane size due to more significant rippling.
The tangent elastic modulus of graphene depends on strain (Fig. 7d). Subject to a moderately large tensile strain (�1%),the anharmonic effect on rippling is significantly reduced, and as a result the harmonic analysis could be used to predict thetemperature/size-dependence of elastic modulus. As shown in Fig. 9a, the tangent biaxial modulus at 1% strain decreaseswith increasing temperature for a graphene membrane with L0¼20 nm, in close agreement with the linear dependencepredicted by the harmonic analysis. Note that, due to the intrinsic nonlinear elasticity, the biaxial modulus in the groundstate (En) has to be adjusted to the value at 1% strain (�353.6 N/m) for the harmonic analysis. Again, 2D-MD simulationspredict a biaxial modulus independent of temperature. The size dependence of the tangent modulus at 1% strain is shown inFig. 9b. The elastic modulus drops rapidly from the ground-state value (353.6 N/m) to a constant level for L042 nm at eachtemperature. As predicted by the harmonic analysis, the size dependence becomes negligible when ε0L
L0b1:6 nm for ε0 ¼ 1%.Finally, as one application, we consider a graphene membrane suspended over a square hole on a substrate. As the
temperature increases from 300 K to 1000 K, thermal expansion of the substrate imposes a positive equi-biaxial strain to themembrane, ε¼ αsΔT , where αs is the CTE of the substrate (assumed to be a constant). As a result, rippling of the suspendedgraphene membrane is subjected to two competing effects: increasing temperature and strain. As shown in Fig. 10a, by MDsimulations, the change of rippling amplitude for the suspended graphene depends on the CTE of the substrate. With arelatively large substrate CTE, the ripple amplitude decreases with increasing temperature, in contrast to the cases witheither zero strain or zero stress (Fig. 5a). Experimental evidence for decreasing membrane roughness with increasingtemperature has been reported by Kirilenko et al. (2011). Moreover, an equi-biaxial stress is induced in the suspendedgraphene membrane due to mismatch in thermal expansion. The stress changes with temperature as follows:
¼ ~Enðαs�αgÞ: ð45Þ
For the graphene membrane, both the CTE (αg) and the biaxial modulus ( ~En
) depend on the temperature and stress.Therefore, integration of Eq. (45) would in general lead to a nonlinear dependence of the thermal stress on temperature. Theresults from MD simulations are shown in Fig. 10b. Assuming zero strain (relative to the ground state) at T¼300 K, themembrane is subjected to an initial tensile stress of 0.1 N/m. Under the zero strain condition (αs ¼ 0), the stress decreasesslightly as the temperature increases, because the CTE of graphene becomes positive at high temperatures (Fig. 6c). Withαs40, the stress increases with temperature nonlinearly. On the other hand, using the thermomechanical properties ofgraphene at 300 K in Eq. (45), the linear prediction (dashed lines) considerably overestimates the stress at hightemperatures (4400 K).
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–58 57
We present a statistical mechanics analysis and molecular dynamics simulations of monolayer graphene membranesunder a variety of thermomechanical conditions. Comparison between the two approaches highlights significantanharmonic effects on rippling and thermoelasticity of graphene. The main findings are summarized as follows.
�The amplitude of thermal rippling depends nonlinearly on the graphene membrane size due to anharmonic interactionsbetween bending and stretching modes. Different roughness exponents are predicted for a power-law scaling under zerostress and zero strain conditions. However, a small positive pre-strain could suppress rippling amplitude considerablyand result in very different scaling behavior.
�Negative in-plane thermal expansion of graphene is predicted at relatively low temperatures, with a transition to positivethermal expansion at high temperatures. The transition is a result of two competing effects: positive thermal expansiondue to in-plane modes and negative expansion due to out-of-plane fluctuation. The latter is suppressed by theanharmonic effect at high temperatures.
�The biaxial stress–strain relation of graphene is generally nonlinear at a finite temperature, even for an infinitesimalstrain. It is found that the tangent biaxial modulus of graphene depends on strain non-monotonically, with strainstiffening followed by intrinsic softening. With an entropic contribution due to rippling, the elastic modulus of graphenedepends on both temperature and membrane size.
�Finally, for a suspended graphene membrane, the ripple amplitude may increase or decrease with increasingtemperature, depending on the coefficient of thermal expansion of the substrate.
The authors gratefully acknowledge financial support of this work by the National Science Foundation through Grant nos.CMMI-0926851 and CMMI-1130261. The authors thank Dr. L.B. Freund of University of Illinois at Urbana-Champaign forhelpful discussions. The authors acknowledge the Texas Advanced Computing Center (TACC) at the University of Texas atAustin for providing HPC resources that have contributed to the research results reported within this paper.
Abedpour, N., Neek-Amal, M., Asgari, R., Shahbazi, F., Nafari, N., Tabar, M.R.R., 2007. Roughness of undoped graphene and its short-range induced gaugefield. Phys. Rev. B 76, 195407.
Abraham, F.F., Nelson, D.R., 1990. Fluctuations in the flat and collapsed phases of polymerized membranes. J. Phys. (Paris) 51 (23), 2653–2672.Admal, N.C., Tadmor, E.B., 2010. A unified interpretation of stress in molecular systems. J. Elast. 100 (1), 63–143.Arroyo, M., Belytschko, T., 2002. An atomistic-based finite deformation membrane for single layer crystalline films. J. Mech. Phys. Solids 50 (9), 1941–1977.Ashcroft, N.W., Mermin, N.D., 1976. Solid State Physics. Cengage Learning, Brooks/Cole.Bangert, U., Gass, M.H., Bleloch, A.L., Nair, R.R., Geim, A.K., 2009. Manifestation of ripples in free-standing graphene in lattice images obtained in an
aberration-corrected scanning transmission electron microscope. Phys. Status Solidi A 206 (6), 1117–1122.Bao, W., Miao, F., Chen, Z., Zhang, H., Jang, W., Dames, C., Lau, C.N., 2009. Controlled ripple texturing of suspended graphene and ultrathin graphite
membranes. Nat. Nanotechnol. 4 (9), 562–566.Bowick, M.J., Travesset, A., 2001. The statistical mechanics of membranes. Phys. Rep. 344 (4), 255–308.Brenner, D.W., Shenderova, O.A., Harrison, J.A., Stuart, S.J., Ni, B., Sinnott, S.B., 2002. A second-generation reactive empirical bond order (REBO) potential
energy expression for hydrocarbons. J. Phys.: Condens. Matter 14 (4), 783–802.Bunch, J.S., Verbridge, S.S., Alden, J.S., van der Zande, A.M., Parpia, J.M., Craighead, H.G., McEuen, P.L., 2008. Impermeable atomic membranes from graphene
sheets. Nano Lett. 8, 2458–2462.Chen, S., Chrzan, D., 2011. Monte carlo simulation of temperature-dependent elastic properties of graphene. Phys. Rev. B 84 (19), 195409.Fasolino, A., Los, J., Katsnelson, M., 2007. Intrinsic ripples in graphene. Nat. Mater. 6 (11), 858–861.Freund, L.B., 2013. Entropic pressure between biomembranes in a periodic stack due to thermal fluctuations. Proc. Natl. Acad. Sci. 110, 2047–2051.Gompper, G., Kroll, D., 1992. Edge correlations of fluid and tethered membranes. J. Phys. I (France) 2 (5), 663–676.Helfrich, W., 1973. Elastic properties of lipid bilayers: theory and possible experiments. Z. Naturforsch. C 28 (11), 693–703.Helfrich, W., Servuss, R.M., 1984. Undulations, steric interaction and cohesion of fluid membranes. Il Nuovo Cimento D 3, 137–151.Humphrey, W., Dalke, A., Schulten, K., 1996. VMD – Visual Molecular Dynamics. J. Mol. Graphics 14, 33–38.Jiang, J., Wang, J., Li, B., 2009. Thermal expansion in single-walled carbon nanotubes and graphene: nonequilibrium green's function approach. Phys. Rev. B
80 (20), 205429.Kammler, D.W., 2007. A First Course in Fourier Analysis. Cambridge University Press, New York.Kirilenko, D.A., Dideykin, A.T., Van Tendeloo, G., 2011. Measuring the corrugation amplitude of suspended and supported graphene. Phys. Rev. B 84 (23),
235417.Koskinen, P., Kit, O.O., 2010. Approximate modeling of spherical membranes. Phys. Rev. B 82 (23), 235420.Kownacki, J.-P., Mouhanna, D., 2009. Crumpling transition and flat phase of polymerized phantom membranes. Phys. Rev. E 79, 040101 (R).Kudin, K.N., Scuseria, G.E., Yakobson, B.I., 2001. C2F, BN, and C nanoshell elasticity from ab initio computations. Phys. Rev. B 64, 235406.Le Doussal, P., Radzihovsky, L., 1992. Self-consistent theory of polymerized membranes. Phys. Rev. Lett. 69 (8), 1209–1212.Lee, C., Wei, X., Kysar, J.W., Hone, J., 2008. Measurement of the elastic properties and intrinsic strength of monolayer graphene. Science 321 (5887), 385–388.Lipowsky, R., Girardet, M., 1990. Shape fluctuations of polymerized or solidlike membranes. Phy. Rev. Lett. 65 (23), 2893–2896.Lomholt, M.A., Loubet, B., Ipsen, J.H., 2011. Elastic moderation of intrinsically applied tension in lipid membranes. Phys. Rev. E 83, 011913.Los, J.H., Katsnelson, M.I., Yazyev, O.V., Zakharchenko, K.V., Fasolino, A., 2009. Scaling properties of flexible membranes from atomistic simulations:
application to graphene. Phys. Rev. B 80 (12), 121405.Lu, Q., Arroyo, M., Huang, R., 2009. Elastic bending modulus of monolayer graphene. J. Phys. D: Appl. Phys. 42 (10), 102002.
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 42–5858
Lu, Q., Gao, W., Huang, R., 2011. Atomistic simulation and continuum modeling of graphene nanoribbons under uniaxial tension. Model. Simul. Mater. Sci.Eng. 19 (5), 054006.
Lu, Q., Huang, R., 2009. Nonlinear mechanics of single-atomic-layer graphene sheets. Int. J. Appl. Mech. 1, 443–467.Lu, Z., Dunn, M.L., 2010. van der Waals adhesion of graphene membranes. J. Appl. Phys. 107 (4), 044301.Marko, J.F., Siggia, E.D., 1995. Stretching DNA. Macromolecules 28 (26), 8759–8770.Meyer, J., Geim, A., Katsnelson, M., Novoselov, K., Booth, T., Roth, S., 2007. The structure of suspended graphene sheets. Nature 446 (7131), 60–63.Mounet, N., Marzari, N., 2005. First-principles determination of the structural, vibrational and thermodynamic properties of diamond, graphite, and
derivatives. Phys. Rev. B 71 (20), 205214.Nelson, D.R., Peliti, L., 1987. Fluctuations in membranes with crystalline and hexatic order. J. Phys. 48 (7), 1085–1092.Nelson, D.R., Piran, T., Weinberg, S., 2004. Statistical Mechanics of Membranes and Surfaces, 2nd ed. World Scientific Publishing Co., Singapore.Pathria, R.K., 1996. Statistical Mechanics, 2nd ed. Butterworth-Heineman, Oxford.Plimpton, S., 1995. Fast parallel algorithms for short-range molecular dynamics. J. Comput. Phys. 117 (1), 1–19.Pozzo, M., Alfè, D., Lacovig, P., Hofmann, P., Lizzit, S., Baraldi, A., 2011. Thermal expansion of supported and freestanding graphene: lattice constant versus
interatomic distance. Phys. Rev. Lett. 106 (13), 135501.Safran, S.A., 1994. Statistical Thermodynamics of Surfaces, Interfaces, and Membranes. Addison-Wesley Pub., Reading, MA.Singh, V., Sengupta, S., Solanki, H.S., Dhall, R., Allain, A., Dhara, S., Pant, P., Deshmukh, M.M., 2010. Probing thermal expansion of graphene and modal
dispersion at low-temperature using graphene nanoelectromechanical systems resonators. Nanotechnology 21 (16), 165204.Su, T., Purohit, P.K., 2012. Semiflexible filament networks viewed as fluctuating beam-frames. Soft Matter 8, 4664–4674.Thompson-Flagg, R.C., Moura, M.J., Marder, M., 2009. Rippling of graphene. Europhys. Lett. 85 (4), 46002.Timoshenko, S., Woinowsky-Krieger, S., 1987. Theory of Plates and Shells, 2nd ed. McGraw-Hill, New York.Treloar, L.R.G., 1958. The Physics of Rubber Elasticity. Oxford University Press, New York.Tuckerman, M., Berne, B.J., Martyna, G.J., 1992. Reversible multiple time scale molecular dynamics. J. Chem. Phys. 97, 1990–2001.Wei, X., Fragneaud, B., Marianetti, C., Kysar, J., 2009. Nonlinear elastic behavior of graphene: ab initio calculations to continuum description. Phys. Rev. B 80
(20), 205407.Wei, Y., Wang, B., Wu, J., Yang, R., Dunn, M.L., 2012. Bending rigidity and Gaussian bending stiffness of single-layered graphene. Nano Lett. 13 (1), 26–30.Weiner, J.H., 2002. Statistical Mechanics of Elasticity. Dover Publications, Mineola, New York.Zakharchenko, K.V, Katsnelson, M., Fasolino, A., 2009. Finite temperature lattice properties of graphene beyond the quasiharmonic approximation. Phys.
Rev. Lett. 102 (4), 046808.Zakharchenko, K.V., Roldán, R., Fasolino, A., Katsnelson, M.I., 2010. Self-consistent screening approximation for flexible membranes: application to
graphene. Phys. Rev. B 82 (12), 125435.Zan, R., Muryn, C., Bangert, U., Mattocks, P., Wincott, P., Vaughan, D., Li, X., Colombo, L., Ruoff, R.S., Hamilton, B., Novoselov, K.S., 2012. Scanning tunnelling
microscopy of suspended graphene. Nanoscale 4 (10), 3065–3068.Zhao, H., Aluru, N., 2010. Temperature and strain-rate dependent fracture strength of graphene. J. Appl. Phys. 108 (6), 064321.